Download presentation

Presentation is loading. Please wait.

Published byKiersten Reavis Modified over 2 years ago

1
Computational Materials Science and Engineering Ab-initio Assisted Process and Device Simulation for Nanoelectronic Devices Wolfgang Windl MSE, The Ohio State University, Columbus, OH, USA 800 o C 20 min As impl. SIMS Model I V

2
Computational Materials Science and Engineering Gate Semiconductor Devices – MOSFET P: holes, e.g. B (Acceptor) N: e -, e.g. As (Donor) Source P Drain P N – V D – V G IDID Gate (Me) Drain P Channel N Insulator (SiO 2 ) – V D 0VG0VG Si Metal Oxide Semiconductor Field Effect Transistor + Analog: Amplification Digital: Logic gates Doping: - Source P Spacer Si

3
Computational Materials Science and Engineering 1. Semiconductor Technology Scaling – Improving Traditional TCAD Feature size shrinks on average by 12% p.a.; speed size Chip size increases on average by 2.3% p.a. Overall performance: by ~55% p.a. or ~ doubling every 18 months (Moores Law)

4
Computational Materials Science and Engineering Bacterium Virus Protein molecule Atom Semiconductor Technology Scaling – Gate Oxide Gate (Me) Drain P Channel N Gate oxide (SiO 2 ) – V D 0VG0VG Si + - Source P C = A/d

5
Computational Materials Science and Engineering Role of Ab-Initio Methods on Nanoscale 1.Improving traditional (continuum) process modeling to include nanoscale effects –Identify relevant equations & parameters (physics) –Basis for atomistic process modeling (Monte Carlo, MD) 2.Nanoscale characterization = Combination of experiment & ab-initio calculations 3.Atomic-level process + transport modeling = structure-property relationship (ultimate goal)

6
Computational Materials Science and Engineering 1. Nanoscale Problems – Traditional MOS What you expect: Intrinsic diffusion 800 °C 20 min 800 °C 1 month 800 °C 20 min What you get: fast diffusion (TED) immobile peak segregation Active B¯

7
Computational Materials Science and Engineering Bridging the Length Scales: Ab-Initio to Continuum Need to calculate: Diffusion prefactors (Uberuaga et al., phys. stat. sol. 02) Migration barriers (Windl et al., PRL 99) Capture radii (Beardmore et al., Proc. ICCN 02) Binding energies (Liu et al., APL 00)

8
Computational Materials Science and Engineering 2. The Nanoscale Characterization Problem Traditional characterization techniques, e.g.: –SIMS (average dopant distribution) –TEM (interface quality; atomic-column information) Missing: Single-atom information –Exact interface (contact) structure (previous; next) –Atom-by-atom dopant distribution (strong V T shifts) New approach: atomic-scale characterization (TEM) plus modeling

9
Computational Materials Science and Engineering Si 0 Si 2+ Si 4+ Si 0 Si 1,2,3+ Si 4+ Abrupt vs. Diffuse Interface AbruptGraded Buczko et al. How do we know? What does it mean?

10
Computational Materials Science and Engineering Z=31 Z=31 Z=33 Z=33 Atomic Resolution Z-Contrast Imaging GaAs EELS Spectrometer EELS Spectrometer < 0.1 nm < 0.1 nmScanningProbe Computational Materials Science and Engineering 1.4Å As Ga

11
Computational Materials Science and Engineering Electron Energy-Loss Spectrum energy loss (eV) intensity (a.u.) ZERO LOSS silicon with surface oxide and carbon contamination LOSS VALENCE x25 optical properties and electronic structure concentration CORE LOSS bonding and oxidation state x500x5000 Si-L C-K O-K VB CB Core hole Z+1

12
Computational Materials Science and Engineering Theoretical Methods ab initio Density Functional Theory plus LDA or GGA implemented within pseudopotential and full-potential (all electron) methods

13
Computational Materials Science and Engineering site and momentumresolvedDOS EFEF conduction band minimum 1s 1/2 2p 3/2 2p 1/2 2s 1/2 energy ground state of Si atom with total energy E 0 excited Si atom with total energy E 1 ~ 90eV ~ 115eV Transition energy E T = E 1 - E 0 E T = ~100 eV 2p 6 2p 5 Si-L 2,3 Ionization Edge in EELS

14
Computational Materials Science and Engineering Calculated Si-L 2,3 Edges at Si/SiO Energy-loss, eV Si Si 4+ Si 1+ Si 2+ Si 3+

15
Computational Materials Science and Engineering Combining Theory and Experiment Si Si 0.5 nm 0.5 nm Energy-loss (eV) Energy-loss (eV) Si - L 2,3 Si - L 2,3 Intensity Intensity Calculation of EELS Spectra from Band Structure

16
Computational Materials Science and Engineering Combining Theory and Experiment Si Si 0.5 nm 0.5 nm Energy-loss (eV) Energy-loss (eV) Si - L 2,3 Si - L 2,3 Intensity Intensity Calculation of EELS Spectra from Band Structure Si 0 Si 1+ Si 2+ Si 3+ Si Fractions Measure atomic structure of amorphous materials.

17
Computational Materials Science and Engineering Band Line-Up Si/SiO 2 Abrupt would be better! Is there an abrupt interface? Lopatin et al., submitted to PRL Real-space band structure: Calculate electron DOS projected on atoms Average layers

18
Computational Materials Science and Engineering Interfaces with Different Abruptness: Si/SiO 2 vs. Si:Ge/SiO 2 Yes! Ge-implanted sample from ORNL (1989). Sample history: Ge implanted into Si (10 16 cm -2, 100 keV) ~ 800 o C oxidation Initial Ge distribution ~120 nm ~4%

19
Computational Materials Science and Engineering Ge after oxidation packed into compact layer, ~ 4-5 nm wide Z-Contrast Ge/SiO 2 Interface Si Si SiO 2 Ge nm Intensity peak ~100% Ge

20
Computational Materials Science and Engineering Kinetic Monte Carlo Ox. Modeling Simulation Algorithm for oxidation of Si:Ge: –Si lattice with O added between Si atoms –Addition of O atoms and hopping of Ge positions by KMC* –First-principles calculation of simplified energy expression as function of bonds: *Hopping rate Ge: McVay, PRB 9 (74); ox rate SiGe: Paine, JAP 70 (91). Windl et al., J. Comput. Theor. Nanosci.

21
Computational Materials Science and Engineering Depth (cm) Concentration (cm -3 ) O Ge Si not shown nm 3 Monte Carlo Results - Animation Ge conc. O conc.

22
Computational Materials Science and Engineering Initial Ge distribution 25 min, 1000 o C Monte Carlo Results - Profiles oxide

23
Computational Materials Science and Engineering Energy-loss (eV) Energy-loss (eV) nm 0.5 nm Ge Ge Si - L 2,3 Si - L 2,3 Intensity Intensity Si Si 0.5 nm 0.5 nm Energy-loss (eV) Energy-loss (eV) Si - L 2,3 Si - L 2,3 Intensity Intensity Si/SiO 2 vs. Ge/SiO 2 Atomic Resolution EELS S. Lopatin et al., Microscopy and Microanalysis, San Antonio, oxide SiGe

24
Computational Materials Science and Engineering Band Line-Up Si/SiO 2 & Ge/SiO 2 Lopatin et al., submitted to PRL

25
Computational Materials Science and Engineering Conclusions 2 Atomic-scale characterization is possible: Ab-initio methods in conjunction with Z-contrast & EELS can resolve interface structure. Atomically sharp Ge/SiO 2 interface observed Reliable structure-property relationship for well characterized structure (band line-up) Abrupt is good Sharp interface from Ge-O repulsion (snowplowing)

26
Computational Materials Science and Engineering Wind et al., JVST B, Possibilities: Carbon nanotubes (CNTs) as channels in field effect transistors Single molecules to function as devices Molecular wires to connect device molecules Single-molecule circuits where devices and interconnects are integrated into one large molecule 3. Process and Device Simulation of Molecular Devices 300 nm

27
Computational Materials Science and Engineering device Concept of Ab-Initio Device Simulation Zhang, Fonseca, Demkov, Phys Stat Sol (b), 233, 70 (2002) Using Landauer formula for I p (V) Lippmann-Schwinger equation, T lr (E) = l V + VGV r Rigid-band approximation T(E,V) = T(E + V) with = 0.5

28
Computational Materials Science and Engineering T lr from Local-Orbital Hamiltonian device (H d ) right elec. (H r ) T l T dl T dr T r left elec. (H l )... Zhang, Fonseca, Demkov, Phys Stat Sol (b), 233, 70 (2002) T lr (E) can be constructed from matrix elements of DFT tight- binding Hamiltonian H. Pseudo atomic orbitals: (r > r c )=0. We use matrix-element output from SIESTA.

29
Computational Materials Science and Engineering The Molecular Transport Problem I Expt. Theor. Strong discrepancy expt.-theory! Suspected Problems: Contact formation molecule/lead not understood Influence of contact structure on electronic properties

30
Computational Materials Science and Engineering What is Process Modeling for Molecular Devices? Contact formation: need to follow influence of temperature etc. on evolution of contact. Molecular level: atom by atom Molecular Dynamics Problem: MD may never get to relevant time scales Accessible simulated time * s ms s ns Year Moores law * 1-week simulation of 1000-atom metal system, EAM potential

31
Computational Materials Science and Engineering Possible solution: accelerated dynamics methods. Principle: run for t run. Simulated time: t sim = n t run, n >> 1 Possible methods: Hyperdynamics (1997) Parallel Replica Dynamics (1998) Temperature Accelerated Dynamics (2000) Accelerated Molecular Dynamics Methods Voter et al., Annu. Rev. Mater. Res. 32, 321 (2002).

32
Computational Materials Science and Engineering Concept: Raise temperature of system to make events occur more frequently. Run several (many) times. Pick randomly event that should have occurred first at the lower temperature. Basic assumption (among others): Harmonic transition state theory (Arrhenius behavior) w/ E from Nudged Elastic Band Method (see above). Temperature Accelerated Dynamics (TAD) Voter et al., Annu. Rev. Mater. Res. 32, 321 (2002).

33
Computational Materials Science and Engineering Carbon Nanotube on Pt From work function, Pt possible lead candidate. Structure relaxed with VASP. Very small relaxations of Pt suggest little wetting between CNT and Pt ( bad contact!?).

34
Computational Materials Science and Engineering Nordlund empirical potential Not much interaction observed study different system. Movie: Carbon Nanotube on Pt Temperature-Accelerated MD at 300 K t sim = 200 s

35
Computational Materials Science and Engineering Carbon Nanotube on Ti Large relaxations of Ti suggest strong reaction (wetting) between CNT and Ti. Run ab-initio TAD for CNT on Ti (no empirical potential available). Very strong reconstruction of contacts observed.

36
Computational Materials Science and Engineering TAD MD for CNT/Ti 600 K, 0.8 ps t sim (300 K) = 0.25 s CNT bonds break on top of Ti, very different contact structure. New structure 10 eV lower in energy.

37
Computational Materials Science and Engineering Contact Dependence of I-V Curve for CNT on Ti Difference 15-20%

38
Computational Materials Science and Engineering Relaxed CNT on Ti Inline Structure In real devices, CNT embedded into contact. Maybe major conduction through ends of CNT?

39
Computational Materials Science and Engineering Contact Dependence of I-V Curve for CNT on Ti Inline structure has 10x conductivity of on-top structure

40
Computational Materials Science and Engineering Currently major challenge for molecular devices: contacts Contact formation: Process modeling on MD basis. Accelerated MD Empirical potentials instead of ab initio when possible Major pathways of current flow through ends of CNT Conclusions

41
Computational Materials Science and Engineering Funding Semiconductor Research Corporation NSF-Europe Ohio Supercomputer Center

42
Computational Materials Science and Engineering Acknowledgments (order of appearance) Dr. Roland Stumpf (SNL; B diffusion) Dr. Marius Bunea and Prof. Scott Dunham (B diffusion) Dr. Xiang-Yang Liu (Motorola/RPI; BICs) Dr. Leonardo Fonseca (Freescale; CNT transport) Karthik Ravichandran (OSU; CNT/Ti) Dr. Blas Uberuaga (LANL; CNT/Pt-TAD) Prof. Gerd Duscher (NCSU; TEM) Tao Liang (OSU; Ge/SiO 2 ) Sergei Lopatin (NCSU; TEM)

43
Left: Ti below 25 a.u. and above 55 a.u. CNT (armchair (3,3), 12 C planes) in the middle Right: Ti below 10 a.u. and above 60 a.u. CNT (3,3), 19 C planes, in contact with Ti between 15 a.u. and 30 a.u. and between 45 a.u. and 60 a.u. CNT on vacuum between 30 a.u. and 45 a.u.

44
Minimal basis set used (SZ); I did a separate calculation for an isolated CNT(3,3) and obtained a band gap of 1.76 eV (SZ) and 1.49 eV (DZP). Armchair CNTs are metallic; to close the gap we need kpts in the z-direction.

45
Notice the difference in the y- axis. The X structure (below) carries a current which is about one order of magnitude smaller than the CNT inline with the contacts (left) The main peak in the X structure is located at ~5 V, which is close to the value from the inline structure (~5.5 V). This indicates that the qualitative features in the conductance derive from the CNT while the magnitude of the conductance is set by the contacts. The extra peaks seen on the right may be due to incomplete relaxation.

46
Notice the difference in the y- axis. The X structure (below) carries a current which is about one order of magnitude smaller than the CNT inline with the contacts (left) The main peak in the X structure is located at ~5 V, which is close to the value from the inline structure (~5.5 V). This indicates that the qualitative features in the conductance derive from the CNT while the magnitude of the conductance is set by the contacts. The extra peaks seen on the right may be due to incomplete relaxation.

47
Current (A)

48
PDOS for the relaxed CNT in line with contacts. The two curves correspond to projections on atoms far away from the two interfaces. A (3,3) CNT is metallic, still there is a gap of about 4 eV. Does the gap above result from interactions with the slabs or from lack of kpts along z? This question is not so important since the Fermi level is deep into the CNT valence band.

49
Previous calculations and new ones. Black is unrelaxed but converged with Siesta while blue is relaxed with Vasp and converged with Siesta. From your results it looks like you started from an unrelaxed structure and is trying to converge it.

50
Current (A) Bias (V) Previous calculations and new ones. Black is relaxed with Vasp and converged with Siesta.

51
MD smoothes out most of the conductance peaks calculated without MD. However, the overall effect of MD does not seem to be very important. That is an important result because it tells us that the Schottky barrier is extremely important for the device characteristics but interface defects are not. Transport seems to average out the defects generated with MD. Notice in the lower plot that there is no exponential regime, indicating ohmic behavior. Slide 7 shows that for the aligned structure the tunneling regime is very clear up to ~6 V.

52
Computational Materials Science and Engineering Ab Initio: Diffusion parameters, stress dependence, etc. Device modeling compare modeled results to specs. Met done, otherwise goto 1. Diffusion Solver - read in implant - solve diffusion Relate atomistic calculations to macroscopic eqs. Physical Multiscale Process Modeling REED-MD Implant: ab-initio modeling (3D dopant distribution)

53
Computational Materials Science and Engineering MOSFET Scaling: Ultrashallow Junctions *P. Packan, MRS Bulletin Higher Doping To get enough current with shallow source & drain Shallower Implant Better insulation (off)

54
Computational Materials Science and Engineering Implantation & Diffusion Channel *Hoechbauer, Nastasi, Windl Dopants inserted by ion implantation damage Damage healed by annealing During annealing, dopants diffuse fast (assisted by defects) important to optimize anneal SourceDrain Gate *

55
Computational Materials Science and Engineering l Coordinates and types of group of atoms (molecule, crystal, crystal + defect, etc.) Solve quantum mechanical Schrödinger equation, H E total energy of system l Calculate forces on atoms, update positions equilibrium configuration thermal motion (MD), vibrational properties Input: Output: H O H H O H Ab-Initio Calculations – Standard Codes

56
Computational Materials Science and Engineering real DFT effective potential Ab-Initio Calculations Everybodys choice: Ab-initio code VASP (Technische Universität Wien), LDA and GGA Error from effective potential corrected by (exchange-)correlation term Local Density Approximation (LDA) Generalized-Gradient Approximations (GGAs) Others (Exact exchange, hybrid functionals etc.) Correct one!?

57
Computational Materials Science and Engineering How To Find Migration Barriers I E ~ 0.4 eV E Energy Easy: Can guess final state & diffusion path (e.g. vacancy diffusion) By hand, drag method. Extensive use in the past. Unreliable! Fails even for exchange N-V in Si (detour lowers barrier by ~2 eV) drag real

58
Computational Materials Science and Engineering How To Find Migration Barriers II New reliable search methods for diffusion paths exist like: Nudged elastic band method (Jónsson et al.). Used in this work. Dimer method (Henkelman et al.) MD (usually too slow); but can do accelerated MD (Voter) All in VASP, easy to use. a b c Elastic band method: Minimize energy of all snapshots plus spring terms, E chain : Initial Saddle Final

59
Computational Materials Science and Engineering Vineyard theory From vibrational frequencies Calculation of Diffusion Prefactors E Energy A S B A S B Phonon calculation in VASP Download our scripts from Johnsson group website (UW)

60
Computational Materials Science and Engineering W. Windl, M.M. Bunea, R. Stumpf, S.T. Dunham, and M.P. Masquelier, Proc. MSM99 (Cambridge, MA, 1999), p. 369; MRS Proc. 568, 91 (1999); Phys. Rev. Lett. 83, 4345 (1999). Reason for TED: Implant Damage NEBM-DFT: Interstitial assisted two-step mechanism: Intrinsic diffusion: Create interstitial, B captures interstitial, diffuse together Diffusion barrier: E form (I) – E bind (BI) + E mig (BI) 4 eV 1 eV 0.6 eV ~ 3.6 eV After implant: Interstitials for free transient enhanced diffusion

61
Computational Materials Science and Engineering Reason for Deactivation – Si-B Phase Diagram Si Si 1.8 B 5.2 Si 10 B B Si B SiB 14 L T( o C)

62
Computational Materials Science and Engineering *S. Solmi et al., JAP 88, 4547 (2000). Deactivation – Sub-Microscopic Clusters Experimental findings: Structures too small to be seen in EM only few atoms New phase nucleates, but decays quickly Clustering dependent on B concentration and interstitial concentration formation of B m I n clusters postulated; experimental estimate: m / n ~ 1.5* Approach: Calculate clustering energies from first principles up to max. m, n Build continuum or atomistic kinetic-Monte Carlo model

63
Computational Materials Science and Engineering Cluster Formation – Reaction Barriers Dimer study of the breakup of B 3 I 2 into B 2 I and BI showed:* BIC reactions diffusion limited Reaction barrier can be well approximated by difference in formation energies plus migration energy of mobile species. *Uberuaga, Windl et al.

64
Computational Materials Science and Engineering B-I Cluster Structures from Ab Initio Calculations B3I20B3I20 B2I0B2I0 BI + BI 2 0 BI 3 + B4I3-B4I3- B3I-B3I- B4I20B4I20 B 4 I 2- B3I3-B3I3- B2I20B2I20 B2I30B2I30 BxIBxI BxI2BxI2 BxI3BxI3 I>3 B 12 I 7 2- B4I4-B4I4- LDA 0.5 GGA N/A X.-Y. Liu, W. Windl, and M. P. Masquelier, APL 77, 2018 (2000).

65
Computational Materials Science and Engineering Activation and Clusters GGA 30 min anneal, different T (equiv. constant T, varying times) B3I3-B3I3- B3I-B3I-

66
Computational Materials Science and Engineering Sum of small errors in ab-initio exponents has big effect on continuum model refining of ab-initio numbers necessary Use Genetic Algorithm for recalibration Calibration with SIMS Measurements Conc. (cm -3 ) 1025 o C 20 s 650 o C 20 min 30 min o C 20 min Depth ( m) As impl. SIMS Model

67
Computational Materials Science and Engineering Statistical Effects in Nanoelectronics: Why KMC? SIMS *A. Asenov Need to think about exact distribution atomic scale!

68
Computational Materials Science and Engineering Conclusion 1 Atomistic, especially ab-initio, calculations very useful to determine equation set and parameters for physical process modeling. First applications of this virtual fab in semiconductor field. In future, atomistic modeling needed (example: oxidation model later).

69
Computational Materials Science and Engineering CNT Metal lead E o V o Vacuum level Lead CNT Before contact After contact L CNT VB CB EFEF EFEF EFEF B = L – CNT CNT-FET as Schottky Junction Desirable: B = 0 to minimize contact resistance. Metals with right B : Pt, Ti, Pd.

70
Computational Materials Science and Engineering

71
Notice the difference in the y- axis. The X structure (below) carries a current which is about one order of magnitude smaller than the CNT inline with the contacts (left) The main peak in the X structure is located at ~5 V, which is close to the value from the inline structure (~5.5 V). This indicates that the qualitative features in the conductance derive from the CNT while the magnitude of the conductance is set by the contacts. The extra peaks seen on the right may be due to incomplete relaxation.

72
Current (A)

73
PDOS for the relaxed CNT in line with contacts. The two curves correspond to projections on atoms far away from the two interfaces. A (3,3) CNT is metallic, still there is a gap of about 4 eV. Does the gap above result from interactions with the slabs or from lack of kpts along z? This question is not so important since the Fermi level is deep into the CNT valence band.

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google